Crystal growth and magnetic properties of Ln-Mn-Al (Ln=Gd, Yb) compounds of the CaCr2Al10 and ThMn12 structure types
Fulfer, Bradford W.; Haldolaarachchige, Neel; Young, David P.; Chan, Julia Y.; Journal of Solid State Chemistry 194 (2012) 143–150; doi:10.1016/j.jssc.2012.05.002

data_1562928
_publ_section_title
;
 Crystal growth and magnetic properties of Ln-Mn-Al (Ln=Gd, Yb) compounds
 of the CaCr2Al10 and ThMn12 structure types
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              143
_journal_page_last               150
_journal_paper_doi               10.1016/j.jssc.2012.05.002
_journal_volume                  194
_journal_year                    2012
_chemical_formula_sum            'Al9.45 Mn2.55 Yb'
_chemical_formula_weight         567.96
_space_group_IT_number           139
_space_group_name_Hall           '-I 4 2'
_space_group_name_H-M_alt        'I 4/m m m'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_H-M   'I 4/m m m'
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   8.9760(3)
_cell_length_b                   8.9760(3)
_cell_length_c                   5.1110(3)
_cell_measurement_temperature    293(2)
_cell_volume                     411.79(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0194
_diffrn_reflns_av_sigmaI/netI    0.0189
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            656
_diffrn_reflns_theta_full        30.98
_diffrn_reflns_theta_max         30.98
_diffrn_reflns_theta_min         3.21
_exptl_absorpt_coefficient_mu    16.004
_exptl_absorpt_correction_T_max  0.467
_exptl_absorpt_correction_T_min  0.449
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_density_diffrn    4.581
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             513
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.582
_refine_diff_density_min         -1.526
_refine_diff_density_rms         0.190
_refine_ls_extinction_coef       0.0035(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.133
_refine_ls_hydrogen_treatment    .
_refine_ls_matrix_type           full
_refine_ls_number_parameters     17
_refine_ls_number_reflns         216
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.133
_refine_ls_R_factor_all          0.0185
_refine_ls_R_factor_gt           0.0174
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0257P)^2^+0.2980P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0415
_refine_ls_wR_factor_ref         0.0419
_reflns_number_gt                208
_reflns_number_total             216
_reflns_threshold_expression     >2\s(I)
_cod_data_source_file            JSSC-2012-194-143.cif
_cod_data_source_block           bwf046
_cod_database_code               1562928